
==== Front
Materials (Basel)Materials (Basel)materialsMaterials1996-1944MDPI 10.3390/ma13010014materials-13-00014ArticleOne-Pot Sonochemical Synthesis of ZnO Nanoparticles for Photocatalytic Applications, Modelling and Optimization Noman Muhammad Tayyab 12*Petru Michal 1Militký Jiří 2Azeem Musaddaq 2Ashraf Muhammad Azeem 31 Department of Machinery Construction, Institute for Nanomaterials, Advanced Technologies and Innovation, Studentská 1402/2, Technical University of Liberec, 461 17 Liberec, Czech Republic; chase04@example.org Department of Material Engineering, Faculty of Textile Engineering, Studentská 1402/2, Technical University of Liberec, 461 17 Liberec, Czech Republic; chase04@example.org (J.M.); chase04@example.org (M.A.)3 Department of Fibre and Textile Technology, University of Agriculture, Faisalabad 38000, Pakistan; chase04@example.org* Correspondence: chase04@example.org; Tel.: +420-77639630756-55-9602 1 2020 13 1 1756-55-9602 14 12 2019 © 2019 by the authors.2019Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).This present study proposed a successful one pot synthesis of zinc oxide nanoparticles (ZnO NPs) and their optimisation for photocatalytic applications. Zinc chloride (ZnCl2) and sodium hydroxide (NaOH) were selected as chemical reagents for the proposed study. The design of this experiment was based on the reagents' amounts and the ultrasonic irradiations' time. The results regarding scanning electron microscopy (SEM), X-ray diffraction (XRD) and Raman spectroscopy confirmed the presence of ZnO NPs with pure hexagonal wurtzite crystalline structure in all synthesised samples. Photocatalytic activity of the developed samples was evaluated against methylene blue dye solution. The rapid removal of methylene blue dye indicated the higher photocatalytic activity of the developed samples than untreated samples. Moreover, central composite design was utilised for statistical analysis regarding the obtained results. A mathematical model for the optimisation of input conditions was designed to predict the results at any given point. The role of crystallisation on the photocatalytic performance of developed samples was discussed in detail in this novel study.

ZnOultrasonicnanoparticlesphotocatalysisoptimisation
==== Body
1. Introduction
During the past few years, the research on metal oxides, particularly zinc oxide (ZnO), has remarkably increased and gained enormous interest from researchers in chemistry, materials science, physics, medical, textiles and many other fields of science [1,2,3,4,5,6,7,8,9,10,11,12]. ZnO belongs to a family of metal oxide semiconductors. ZnO is an n-type semiconductor with wide band gap (3.37 eV) and having large exciton binding energy (60 meV). On the nanoscale, ZnO shows exceptional physicochemical properties that are beneficial in many industrial applications. Many researchers have successfully used ZnO nanostructures in photocatalytic [13,14,15,16], photovoltaic [17,18,19,20], biomedical [21,22,23,24] and sensing [25,26,27,28,29,30,31] applications, as it provides large surface area as compared to its bulk counterpart. The demand of highly efficient, durable and robust photocatalysts for wastewater treatment makes ZnO nanostructures a reliable candidate for photocatalytic applications.

Researchers have been concluded that the photocatalytic performance of nanomaterials significantly depends upon the synthesis route, size, shape, crystallinity and dimension [32,33,34,35,36]. At present, different researchers have prepared ZnO nanostructures by different synthesis methods i.e., sol–gel [37,38,39], hydrothermal [40,41,42], co-precipitation [43,44,45], green [46,47,48,49], electrospinning [50,51] and sonochemical [52,53]. The sonochemical method among all mentioned methods has been proven to be a more economic, efficient and facile approach used for the synthesis of nanomaterials. This sonochemical method works on the principle of acoustic cavitation. In liquids, ultrasonic energy induces physicochemical changes in a material through low-pressure/high-pressure waves. These waves lead to create a huge number of unstable vacuum bubbles that aggressively collide with each other due to pressure difference, and develop extremely local conditions, i.e., local pressure and temperature raised up to 20 MPa and 5000 K, respectively, with cooling rate 1010 K·s−1 [54]. The size and crystallinity of the synthesised structures have been very well controlled by the sonochemical method, and that is another advantage of using this method.

In an experimental study, Pholnak et al. used an ultrasonic homogeniser as a tool to fabricate ZnO NPs under varying shapes i.e., sphere, cube and cylinder. They sonochemically treated zinc nitrate with hexamethylenetetramine at ambient temperature. They reported that the ultrasonic homogeniser is a better tool for nanomaterials' synthesis than the ultrasonic bath and sonoreactor. Moreover, scanning electron microscopy (SEM) and X-ray diffraction (XRD) results confirmed the formation of ZnO NPs with an average particle size of 70 nm [55]. In another study, Hipolito and Martinez used the sonochemcial method and synthesised ZnO NPs at room temperature and further used them as a photocatalyst in hydrogen gas generation. They reported that the high surface area and smaller particle size of ZnO NPs significantly enhances hydrogen production. Furthermore, they suggested ultrasonic energy an efficient and cost-saving tool, as they used the ultrasonic method for avoiding long reaction time and high temperature [56]. Ma et al. fabricated two-dimensional (2D), hierarchical, fern-like nanoleaves of ZnO in water at room temperature with significantly enhanced photocatalytic performance by this ultrasonic method. The results obtained by different characterisation techniques i.e., SEM, XRD and Transmission electron microscopy (TEM), which confirmed the synthesis of 2D ZnO through the ultrasonic method. They concluded the ultrasonic method as a clean and economic route for large scale production of novel nanostructures [57]. Mahmoodi et al. worked on the modelling of the photocatalytic dye removal of basic blue 41 and basic red 46 by using ZnO NPs, and explained that under optimised conditions the maximum dye removal achieved by ZnO was 72.56% [58]. Dhiman et al. studied the modelling and optimisation of the dye removal efficiency of ZnO NPs by using acridine orange. They used the green chemical method for the synthesis of ZnO NPs and reported a maximum of 72% dye removal efficiency for the synthesised pure ZnO [59]. In another modelling and optimisation study of ZnO, the photocatalytic degradation of RB 19 and RB 21 was investigated by Rodrigues et al. under a UV photoreactor. They obtained 100% dye removal for RB 19, but the time taken for this was more than six hours [60].

In this novel study, ultrasonic homogeniser was used for one pot sonochemical synthesis of ZnO NPs for photocatalytic degradation of methylene blue. This study was conducted to investigate the influence of ultrasonic energy onto the structure and morphology of ZnO NPs, as well as the synergistic role of ZnO NPs onto photocatalytic applications. The process variables i.e., amount of zinc chloride (ZnCl2) and sodium hydroxide (NaOH), and the total time for ultrasonic irradiations, were adjusted by central composite design to attain the optimum conditions. To the best of our knowledge, there is no literature available regarding the synthesis of ZnO in this manner. This work represents a unique demonstration about the modelling and optimisation of as synthesised ZnO. Moreover, regarding the reagents used in this experimental study, it is supposed that this method is a robust one that could be extended for other zinc precursors and synthesis methods.

2. Materials and Methods
2.1. Materials
Zinc chloride (ZnCl2), sodium hydroxide (NaOH), ethanol (C2H5OH) and methylene blue (MB) dye with the chemical formula C16H18ClN3S were received from Sigma-Aldrich (Prague, Czech Republic). The chemicals were used as received.

2.2. Design of Experiment
A Central Composite Design (CCD) is a set of experimental designs with three different design points i.e., factorial points (±1), a centre point (0) and star/axial points (±α). For a three factors CCD, the value of α is 1.68. The general form of a CCD with three input variables/factors (A, B, C) and their coded values (±1), centre point (0) and axial/star points (±α) is illustrated in Figure 1. The CCD is a valuable asset in determining the response surfaces by fitting a quadratic model in order to estimate the effect of curvature, or to find out the maxima or minima of a variable. Table 1 illustrates the input variables (factors) and the factors level setting in their coded form based on CCD.

The design of experiment (DOE) with different amounts of ZnCl2 and NaOH under varying sonication time based on CCD with experimental results is illustrated in Table 2. Some preliminary experiments were conducted to calculate the optimal point of each variable before starting the final experiment. The influence of variables on results was adjusted by using quadratic Equation (1).
 (1) Y=b0+∑ biXi+∑ bi.jXiXj+∑ bi.iXi2   i≥j    i,j=1,2,3 
where b0 is the coefficient of constant term, bi represents the coefficient of linear term, bi.j represents the coefficient of two factors interaction, and bi.i is the coefficient of quadratic term, respectively [54].

2.3. Synthesis of ZnO NPs
In one pot synthesis of zinc oxide nanoparticles (ZnO NPs), varying amounts of ZnCl2 (1.5 g to 18.5 g) were added into a beaker and then we adjusted the amount of water so that the total volume of the solution was maintained at 100 mL. During all experiments, distilled water was utilised. Sonicate the solution for 5 min to make a homogenous solution. A varied amount of NaOH granules (3.3 g to 11.7 g) was added into the running solution. To complete the reaction mechanism, the solution was then sonicated for different time intervals (19.7 min to 70.2 min) based on CCD under ultrasonic probe homogeniser (Bandelin Sonopuls HD 3200, Bandelin Electronic GmbH & Co. KG, Berlin, Germany, 20 kHZ, 200 W, 50% efficiency). The effective power of ultrasonic waves emitted into the solution was 100 Wcm−2, which value was experimentally determined by calorimetric measurement. After the completion of the sonication process, the resulting white flocculates were washed five times with ethanol to remove the excess amount of trashes and impurities. Afterwards, the white flocculates were centrifuged at 4000 rpm for 15 min to separate solid particles from liquid. The centrifuged solid was dried at 80 °C for 1 h in an oven to remove the remaining percentage of moisture and organic impurities. The centrifuged solid was then grinded to obtain the fine powder of ZnO that further characterised it. During our experiments, we observed that Sample 3 provided the maximum MB removal (%). So, in order to compare and to investigate the essential impact of the ultrasonic method, a similar sample was synthesised by the conventional magnetic stirring method under same experimental conditions without sonication, and named as sample M, as provided in Table 2. The schematic illustration of the experimental setup is given in Figure 2.

2.4. Characterisation of ZnO NPs
The surface topography and morphological changes of sonosynthesised ZnO NPs were observed by Ultra High-Resolution Scanning Electron Microscope UHR-SEM Zeiss Ultra Plus (Carl Zeiss Meditec AG, Jena, Germany) with an accelerating voltage of 2 kV. The charging effect was eliminated by the use of a charge compensator (local N2 injection). For the investigation of crystal structure, XRD patterns were collected by an X'Pert PRO X-ray diffractometer (Malvern Panalytical Ltd., Malvern, UK) using Cu Kα radiation of wavelength λ = 0.15406 nm with a scanning angle (2θ) range 5–80° with step size of 0.02° at voltage and current of 40 kV and 30 mA, respectively. The collected patterns were compared with standard patterns of the International Centre for Diffraction Data (ICDD) Powder Diffraction File (PDF: 89-7102) and further analysed. Moreover, Raman spectroscopy (Thermo scientific DXR Raman spectroscope, Thermo Fisher Scientific, Waltham, MA, USA) was utilised to detect the purity of the crystal phase. In order to calculate the size of the crystals, Scherrer's crystallite Equation was used as given below: (2) D=KλβCosθ 

In Equation (2), D represents the crystallite size calculated through line broadening of plane reflection whereas, λ represents the wavelength of the X-ray radiations. β is the full line width at half-maximum height (FWHM) and K represents the shape constant with a constant value i.e., 0.89.

2.5. Photocatalytic Activity of ZnO NPs
Photocatalytic activity of developed samples of ZnO NPs was investigated by photodegradation of MB dye solution under UV light irradiations. For this study, 0.01% (w/v) solution of MB dye was prepared, and 0.5 g·L−1 of the as synthesised nano ZnO (Sample 3 and Sample M) was mixed in running solution. The suspension was kept in the dark for 40 min to reach equilibrium. The suspension was then exposed to a 500 W xenon lamp for 2 h. The distance between the UV lamp and the suspension was 30 cm, and the intensity of the UV light was 20 W·m−2, depending on the distance between the lamp and the sample. After a certain time, an aliquot was taken out and a UV-vis spectrum was recorded on a UV-1600PC Spectrophotometer (VWR International, Radnor, PA, USA). The characteristic concentration peak of MB was obtained at 668 nm of wavelength. The colour removal percentage (CR%) was calculated by the given equation: (3) CR%=[1−CC0]×100 

In Equation (3), C0 and C represents initial and final concentration of MB dye in the solution, respectively.

3. Results and Discussion
3.1. Characterisation of ZnO NPs
The results regarding the surface topography and morphology of synthesised ZnO NPs were collected by SEM micrographs and illustrated in Figure 3. SEM results explained that sonication induced a great impact on the particle size of the resulting ZnO NPs. We observed that crystallite size for Sample 3 is two times smaller than Sample M. For Sample 3, we observed a homogenous distribution and quasi-spherical morphology of ZnO NPs, while an elliptical shape with sharp edges was observed for Sample M. The average particle size for Sample 3 and Sample M was 28 nm and 70 nm, respectively, as calculated from SEM images by ImageJ software (version 1.52p). These results are in good agreement with the findings of our previous investigation in which we concluded that ultrasonic irradiations play a significant role onto the smaller size and morphology of metal oxide nanoparticles [61].

XRD analysis is a valuable asset in order to determine the crystal structure and crystallite size of a samples. The XRD patterns for observed samples (Sample 3 and Sample M) showed that the synthesised ZnO NPs possessed a pure hexagonal wurtzite crystal structure, as all the obtained peaks under XRD analysis for both methods (sonochemical and conventional stirring) matched with the ICDD file (PDF: 89-7102). In Figure 4, the highest peak obtained at 2θ = 36.2° is the characteristic crystalline peak of hexagonal wurtzite crystals of pure ZnO that follows [101] plane reflection. Moreover, a series of crystalline peaks at 2θ = 31.7°, 34.4°, 47.5°, 56.6°, 62.8° and 67.9° follow the [100], [002], [102], [110], [103] and [112] planes, respectively. We observed that hexagonal wurtzite crystals of nano ZnO were formed by both methods with a significant difference regarding crystal size for these methods. The average particle size for observed samples calculated by Scherrer's Equation was 28.1 nm and 70.8 nm for Sample 3 and Sample M, respectively. The average particle size of all the samples prepared by the sonochemical method was 28 nm. The samples prepared by this sonochemical method have three times less particle size than the conventional method, which explains the significant role of the ultrasonic method in the synthesis mechanism of nanomaterials. The XRD results for particle size are in good agreement with the SEM results. Furthermore, no other phase (impurities) i.e., Zn(OH)2, was found during the XRD analysis.

Raman analysis is one of the finest modes for identifying the purity of a crystal lattice or the phase purity of a molecule. The results regarding the Raman analysis for all prepared samples are presented in Figure 5. It was observed that all the Raman bands matched with the characteristic peaks of pure hexagonal wurtzite ZnO. Factor group analysis for vibrational modes of crystals explained that the pure wurtzite crystal phase of ZnO consists of given Raman active modes i.e., (238, 331, 436, 537, 1085 and 1593 cm−1). In Figure 5, a strong peak at 537 cm−1 was observed, which is the metaphor for wurtzite ZnO NPs. Moreover, no characteristic peak of impurity i.e., Zn(OH)2, was found during analysis. The Raman results are significant and consistent with XRD results, and both techniques confirmed the formation of pure hexagonal wurtzite crystal of nano ZnO.

Specific surface area and pore size distribution are significantly influential microstructural properties of ZnO NPs highly dependent upon the geometry, morphology and porosity of as synthesised NPs. These parameters were measured by the Brunauer–Emmet–Teller (BET) method under N2 (−196 °C) atmosphere. The volume of a gas adsorbed is considered as the total area including the specific surface area and pore size. The average specific surface area of ultrasonically prepared samples (Sample 3) was 107 m2·g−1. The experimentally-determined values of surface area, pore volume and pore size distribution of all samples are provided in Table 3.

3.2. Photocatalytic Activity of ZnO NPs
The photocatalytic activity of as synthesised ZnO NPs was evaluated against MB dye solution. 0.5 g·L−1 of the prepared ZnO NPs was used for 50 mg·L−1 of MB dye. It was observed that under UV light irradiations, samples prepared by the ultrasonic method completely degraded MB dye in less than 60 min, while for Sample M, the degradation took a longer time. The results are quite obvious, as we obtained a smaller particle size by the sonochemical method than any conventional method. The results of MB degradation are in good agreement with BET results. The results of MB degradation for Sample 3 and Sample M are illustrated in Figure 6. In order to confirm that MB degradation was only due to ZnO NPs, a controlled sample of MB dye (without ZnO NPs) was exposed to UV light. This sample did not change its colour even after a longer time. This confirmed that MB degradation was only due to the presence of ZnO NPs in the dye solution. The overall results explain that sonochemically-prepared samples showed higher photocatalytic performance for MB than Sample M. UV-vis spectral changes in the MB dye solution as a function of UV light irradiations' times are illustrated in Figure 6.

The ln Ao/A plot for the complete degradation of MB against irradiation time is illustrated in Figure 7, where Ao represents the absorbance at time t = 0 min, and A represents the absorbance after a complete MB degradation at time t = ∞ min. The results explained that in a controlled sample (without ZnO NPs), no change was observed in MB degradation even after longer time, while 53% change was observed for Sample M as it is synthesised by a conventional method. However, a complete 99.9% MB degradation was observed in case of Sample 3. Furthermore, in order to investigate the behaviour of MB under different conditions, i.e., in the presence of dark, in the presence of light, in the presence of Sample M (with and without light) and in the presence of Sample 3 (with and without light), had also been evaluated, and the results are illustrated in Figure 8. Under dark conditions without ZnO NPs, the MB colour remained unchanged. Under irradiations (light conditions) without ZnO NPs, we still did not observe any significant change. For Sample M, 7% and 48% degradation of MB dye was observed under dark and light conditions, respectively. 16% colour change was observed for Sample 3 under dark conditions, whereas a significant colour change of 99.9% was observed for Sample 3 during light irradiations that showed the excellent photocatalytic activity of prepared ZnO NPs. It was noted that the colour change of MB under dark conditions for both samples (Sample M and Sample 3) was only because of the extra white colour of the prepared samples, which means that even with the photocatalyst, the process of photocatalysis was not started without light. So, we concluded that for photocatalytic degradation of pollutants, the presence of both, i.e., light and photocatalyst, is necessary. The influence of the ultrasonic method was significantly high, as we observed 99.9% MB degradation for Sample 3.

Photocatalysis is a dynamic mechanism and the most fundamental property of nano ZnO that triggers a series of oxidation and reduction reactions. In photocatalysis, nano ZnO absorbs light energy and breaks down the long chain organic molecules (pollutants) into smaller fragments i.e., atoms, ions and radicals. Theoretically, photocatalysis is the conversion of light energy into chemical energy to produce radicals and other unstable chemical compounds. The primary oxidizing species formed during photocatalysis are hydroxyl radicals and superoxide anions [62]. The hexagonal wurtzite crystal form of pure ZnO is significantly used in many industrial and practical applications. Rakhshaei et al. reported that ZnO NPs with hexagonal phase show significant photocatalytic properties [63]. When a photon having energy greater than the band gap energy of ZnO strikes on its surface, electrons are released. The released electron further reacted with atmospheric oxygen to become a super oxide anion (O2−). The surface that has lost an electron takes another electron from moisture to fill up the hole. This converted the moisture into a hydroxyl radical (•OH). The two, i.e., the hydroxyl radical (•OH) and the superoxide anion (O2−) are highly reactive, and due to their strong oxidative power, they decompose organic compounds that cause staining. In our previous investigation, we explained the role of reactive oxygen species (ROS) during photocatalysis and reported that hydroxyl radicals (•OH) are the major radical scavengers that are responsible for the degradation of pollutants [56]. More production of ROS on the surface of the photocatalyst increases their power to degrade pollutants. The general mechanism of photocatalysis on the surface of nano ZnO is illustrated in Figure 9.

3.3. Modelling and Optimization
The experimental design (CCD) and response surface plots, i.e., surface plots and contour plots, were analysed to investigate the effects of input variables onto response. In modelling and optimisation, 3D surface plots and the 2D contour plot are helpful to visualise the effect of independent variables onto dependent variables. In total, 20 experimental samples were designed with variation in reagents amount and sonication time as illustrated in Table 2. For better visualisation of the drawn plots and for more accuracy regarding the analysis, Design-Expert 10 was used for statistical analysis. The results presented in Table 2 indicate that the photocatalytic activity of the developed samples increased with an increase in ZnCl2 and NaOH amount up to 15 g and 10 g, respectively. The results showed that MB removal (%) increased from 62.4% to 95.8%, 78.1% to 84.3% and 58.4% to 88.1%, by increasing active reagents amount and sonication time up to their maximum levels. However, the best outcome of 99.3% was achieved with optimal conditions, i.e., ZnCl2 15 g, NaOH 10 g and sonication time 60 min, whereas, the predicted response value for MB removal (%) at optimal conditions (Sample 3) was 99.7%.

A mathematical model (Equation (4)) was suggested to evaluate the obtained results and the relationship between selected variables and response surfaces. The designed response by the model was a function of independent variables. This model is beneficial in the prediction of selected variables at any given point in space. By using this model, response surfaces and contour plots were drawn and analysed, as presented in Figure 10, Figure 11 and Figure 12. MB removal (%) on the basis of the designed model is calculated by the following Equation (4).
 (4) MB Removal (%)=5.26−0.99(ZnCl2)+2.56(NaOH)+2.36(Time)+0.40(ZnCl2×NaOH)+0.02(ZnCl2×Time)−0.09(NaOH×Time)−0.06(ZnCl2)2−0.13(EG)2−0.02(Time)2 

Analysis of variance (ANOVA) was used to examine the interaction of data between selected variables and obtained response from samples 1–20. The results were further analysed to judge the goodness of fit. The results showed that the designed model for MB removal (%) is statistically significant for an F-value of 35.32 and prob > F of <0.0001, as shown in Table 4. R-squared coefficient was used to predict the fit of the model. The results explained that only 3.05% of the total variables cannot be explained by the designed model for MB removal (%). Low coefficient of variation (CV%) values of the developed model explained the precision and accuracy of the results and reliability of the experiment.

A comparison of actual values and predicted values for MB removal (%) is illustrated in Figure 13 that was used to detect the values that were not detected by the designed model. This comparative plot explains the overall pros of our fitted model in terms of statistical analysis and absolute residual minimisation. It was observed that the experimental values were very close to the normal distribution line, indicating a good fit of the model. The normal probability plot of residuals for raw residuals, internally studentised residuals and externally studentised residuals regarding MB degradation, is illustrated in Figure 14 that explained the relationship of experimental data with the standardised normal distribution, whereas the plot between residuals and experimental run order for raw residuals, internally studentised residuals and externally studentised residuals regarding MB degradation is presented in Figure 15, respectively. These graphs explained the lurking factors that influenced the response during experimentation. The optimal design points on the basis of Table 2 and Equation (4) are 15 g ZnCl2, 10 g NaOH and 60 min sonication time.

4. Reusability Performance of ZnO NPs for Sequential Applications
Reusability of ZnO NPs is an essential attribute from the point of sequential application. The reusability performance of Sample 3 (sonochemical method) and Sample M (conventional method) was estimated in the photocatalytic removal of MB for seven reuse cycles. After each cycle, both samples were extracted from their respective solutions by centrifuge process and washed with ethanol and then distilled water, respectively. After drying the samples at 100 °C for 1 h, they were reused again in the fresh MB solution until the seventh cycle. As shown in Figure 16, only a 6.1% MB degradation loss was observed for a sonochemically-prepared sample (Sample 3) even after seven reused cycles, while 26.9% loss was found for the conventional method (Sample M), respectively. Interestingly, the morphology was unchanged before and after each cycle. The overall results regarding the photodegradation and reusability confirmed that the sonochemical method is a facile and durable method for the synthesis of robust and more photocatalytically-active ZnO NPs than the conventional method.

5. Conclusions
ZnO NPs with pure hexagonal wurtzite crystalline structure were successfully synthesised by a one pot sonochemical method using ZnCl2 and NaOH as reactive variables. The samples prepared by the sonochemical method showed a more significantly enhanced photocatalytic performance than the conventional method (Sample M). The average particle size for ZnO NPs prepared by this sonochemical method was three times smaller than for that conventional method (Sample M). Ultrasonic irradiations played a remarkably crucial role in order to synthesise hexagonal wurtzite crystals of nano ZnO with smaller particle size and higher photocatalytic activity as compared to the conventional method. The photo degradation of MB dye recommends the potential use of sonochemically prepared ZnO NPs in waste water treatment for industries, especially the textile industry. Reusability of the prepared ZnO NPs during photocatalytic removal of the MB dye confirmed their durability for industrial applications. The as prepared nano ZnO could be further utilised in many other functional textile applications i.e., self-cleaning and UV protection.

Author Contributions
M.T.N. conceived, designed, performed experiments regarding ZnO NPs and wrote manuscript. M.P. analyzed the results, supervised and acquired funding. J.M. conceived and analyzed the results and make corrections. M.A. performed characterization for synthesized material. M.A.A. performed statistical analysis and reviewed manuscript. All of the authors participated in critical analysis and preparation of the manuscript. All authors have read and agreed to the published version of the manuscript.

Funding
This research work was funded by the Ministry of Education, Youth and Sports of the Czech Republic and the European Union (European Structural and Investment Funds—Operational Programme Research, Development and Education) in the frames of the project "Modular platform for autonomous chassis of specialized electric vehicles for freight and equipment transportation", Reg. No. CZ.02.1.01/0.0/0.0/16_025/0007293.

Conflicts of Interest
The authors declare no conflict of interest.

Figure 1 General form of three factors Central Composite Design (CCD) with coded values.

Figure 2 Graphical representation of sonochemical synthesis of ZnO NPs.

Figure 3 Scanning electron microscopy (SEM) analysis for (a) Sample 3 developed with optimal conditions Zinc chloride (ZnCl2) 15 g, sodium hydroxide (NaOH) 10 g, Sonication time 60 min, (b) Sample M developed without sonication.

Figure 4 XRD pattern for Sample 3 developed with optimal conditions ZnCl2 15 g, NaOH 10 g, Sonication time 60 min, and Sample M developed without sonication.

Figure 5 Raman spectrum for Sample 3 developed with optimal conditions ZnCl2 15 g, NaOH 10 g, Sonication time 60 min, and Sample M developed without sonication.

Figure 6 UV-Vis spectral changes as a function of irradiations time in MB dye solution containing synthesised ZnO (a) Sample 3 developed with optimal conditions ZnCl2 15 g, NaOH 10 g, Sonication time 60 min, (b) Sample M developed without sonication.

Figure 7 Time-dependent photocatalytic removal of MB. Ao show the absorbance at time t = 0, whereas A represents the absorbance at time t = ∞, respectively.

Figure 8 Behaviour of MB degradation under different conditions.

Figure 9 Proposed reaction mechanism on the surface of ZnO NPs for the generation of a reactive oxygen species (ROS).

Figure 10 Response surface and contour plot for MB degradation (%) as a function of ZnCl2 and NaOH where (a) Response surface (b) contour plot respectively.

Figure 11 Response surface and contour plot for MB degradation (%) as a function of ZnCl2 and ultrasonic irradiation time where (a) Response surface (b) contour plot respectively.

Figure 12 Response surface and contour plot for MB degradation (%) as a function of NaOH and ultrasonic irradiation time where (a) Response surface (b) contour plot respectively.

Figure 13 A plot of actual responses vs. predicted responses for MB removal (%).

Figure 14 Normal plot of residuals for (a) raw residuals (b) internally studentized residuals and (c) externally studentized residuals respectively.

Figure 15 The plots of residuals vs. run for (a) raw residuals (b) internally studentized residuals and (c) externally studentized residuals respectively.

Figure 16 Reusability performance of sonochemical method (Sample 3) vs. conventional method (Sample M) as a photocatalysts against MB removal (%).

materials-13-00014-t001_Table 1Table 1 The factors level setting of a 3-factors CCD matrix under coded values for the synthesis of zinc oxide nanoparticles (ZnO NPs).

Experimental Trial	Factors Level Setting	
A	B	C	
1	−1	−1	−1	
2	1	−1	−1	
3	−1	1	−1	
4	1	1	−1	
5	−1	−1	1	
6	1	−1	1	
7	−1	1	1	
8	1	1	1	
9	−α	0	0	
10	α	0	0	
11	0	−α	0	
12	0	α	0	
13	0	0	−α	
14	0	0	α	
15	0	0	0	
16	0	0	0	
17	0	0	0	
18	0	0	0	
19	0	0	0	
20	0	0	0	
materials-13-00014-t002_Table 2Table 2 The 3-factors CCD matrix based on experimental values for actual variables and for experimental and predicted response of methylene blue (MB) removal.

Sample Number	ZnCl2 (g)	NaOH (g)	Sonication Time (min)	MB Removal (%)
Experimental	MB Removal (%)
Predicted	
Sample M	15	10	−	55.3	−	
1	15	5	60	94.6	95.1	
2	10	7.5	19.7	58.4	62.3	
3	15	10	60	99.3	99.7	
4	10	7.5	45	86.6	84.6	
5	5	10	30	65.1	63.0	
6	18.5	7.5	45	95.8	96.7	
7	10	3.3	45	78.1	80.8	
8	10	7.5	45	81.3	84.6	
9	15	5	30	73.4	70.0	
10	10	7.5	45	83.2	84.6	
11	10	7.5	45	87.6	84.6	
12	5	5	60	82.5	81.5	
13	5	10	60	64.3	66.2	
14	1.5	7.5	45	62.4	63.4	
15	10	7.5	45	84.4	84.6	
16	5	5	30	66.4	64.4	
17	10	7.5	45	85.1	84.6	
18	15	10	30	89.2	88.6	
19	10	11.7	45	84.3	83.6	
20	10	7.5	70.2	88.1	86.2	
materials-13-00014-t003_Table 3Table 3 Results of specific surface area and pore volume distribution of ZnO NPs.

Sample No.	Surface Area (m2·g−1)	Pore Volume (cm3·g−1)	Pore Size
(nm)	
Sample M	53	0.51	49	
1	104	0.30	23	
2	105	0.27	21	
3	111	0.20	16	
4	108	0.25	19	
5	107	0.27	19	
6	105	0.28	22	
7	106	0.24	21	
8	108	0.23	19	
9	105	0.26	22	
10	106	0.25	21	
11	107	0.24	20	
12	109	0.21	19	
13	108	0.22	19	
14	106	0.23	21	
15	107	0.26	20	
16	108	0.22	19	
17	106	0.24	22	
18	109	0.20	18	
19	107	0.21	19	
20	108	0.23	18	
materials-13-00014-t004_Table 4Table 4 Analysis of variance (ANOVA) results regarding MB removal (%) for ZnO NPs.

Source	Sum of Squares	df	Mean
Square	F Value	p-Value
Prob > F	Remarks	
Model	2560.20	9	284.47	35.32	<0.0001	Significant	
A-ZnCl2	1322.18	1	1322.18	164.15	<0.0001	Significant	
B-NaOH	9.55	1	9.55	1.19	0.3017	Not significant	
C-Sonication Time	680.84	1	680.84	84.53	<0.0001	Significant	
AB	200.00	1	200.00	24.83	0.0006	Significant	
AC	32.00	1	32.00	3.97	0.0742	Not significant	
BC	98.00	1	98.00	12.17	0.0058	Significant	
A2	36.34	1	36.34	4.51	0.0596	Not significant	
B2	10.26	1	10.26	1.27	0.2855	Not significant	
C2	191.87	1	191.87	23.82	0.0006	Significant	
Residual	80.55	10	8.05	-	-	-	
Lack of Fit	54.47	5	10.89	2.09	0.2191	Not significant	
Pure Error	26.08	5	5.22	-	-	-	
Cor Total	2640.75	19	
	-	-	-	
R-squared: 0.9695, adjusted R-squared: 0.9420, CV%: 3.53.
==== Refs
References
1. Abadi P.G.-S.  Shirazi F.H.  Joshaghani M.  Moghimi H.R.   Ag+-promoted zinc oxide [Zn (O): Ag]: A novel structure for safe protection of human skin against UVA radiation Toxicol. In Vitro 2018 50 318 756-55-9602/j.tiv.2018.02.016 29499336 
2. Ahmad R.  Majhi S.M.  Zhang X.  Swager T.M.  Salama K.N.   Recent progress and perspectives of gas sensors based on vertically oriented ZnO nanomaterials Adv. Colloid Interface Sci. 2019 270 1 27 10.1016/j.cis.2019.05.006 31154073 
3. Appiah-Ntiamoah R.  Baye A.F.  Gadisa B.T.  Abebe M.W.  Kim H.   In-situ prepared ZnO-ZnFe2 O4  with 1-D nanofiber network structure: An effective adsorbent for toxic dye effluent treatment J. Hazard. Mater. 2019 373 459 756-55-9602/j.jhazmat.2019.03.108 30939428 
4. Boscarino S.  Filice S.  Sciuto A.  Libertino S.  Scuderi M.  Galati C.  Scalese S.   Investigation of ZnO-decorated CNTs for UV Light Detection Applications Nanomaterials 2019 9 1756-55-9602/nano9081099 31370341 
5. Buşilă M.  Muşat V.  Textor T.  Mahltig B.   Synthesis and characterization of antimicrobial textile finishing based on Ag: ZnO nanoparticles/chitosan biocomposites RSC Adv. 2015 5 21562 21756-55-9602/C4RA13918F 
6. Costa S.  Ferreira D.  Ferreira A.  Vaz F.  Fangueiro R.   Multifunctional flax fibres based on the combined effect of silver and zinc oxide (Ag/ZnO) nanostructures Nanomaterials 2018 8 1756-55-9602/nano8121069 30572578 
7. Hao N.  Xu Z.  Nie Y.  Jin C.  Closson A.B.  Zhang M.  Zhang J.X.   Microfluidics-enabled rational design of ZnO micro-/nanoparticles with enhanced photocatalysis, cytotoxicity, and piezoelectric properties Chem. Eng. J. 2019 378 122756-55-9602/j.cej.+1-945-404-0451 
8. Iyigundogdu Z.U.  Demir O.  Asutay A.B.  Sahin F.   Developing novel antimicrobial and antiviral textile products Appl. Biochem. Biotechnol. 2017 181 1155 1756-55-9602/s12010-016-2275-5 27734286 
9. Ling C.  Guo T.  Shan M.  Zhao L.  Sui H.  Ma S.  Xue Q.   Oxygen vacancies enhanced photoresponsive performance of ZnO nanoparticles thin film/Si heterojunctions for ultraviolet/infrared photodetector J. Alloys Compd. 2019 797 1224 1756-55-9602/j.jallcom.2019.05.150 
10. Messih M.A.  Shalan A.E.  Sanad M.F.  Ahmed M.   Facile approach to prepare ZnO@ SiO2  nanomaterials for photocatalytic degradation of some organic pollutant models J. Mater. Sci. Mater. Electron. 2756-55-96021 14756-55-9602/s10854-019-01798-9 
11. Norek M.   Approaches to enhance UV light emission in ZnO nanomaterials Curr. Appl. Phys. 2019 19 867 756-55-9602/j.cap.2019.05.006 
12. Rong P.  Ren S.  Yu Q.   Fabrications and Applications of ZnO Nanomaterials in Flexible Functional Devices—A Review Crit. Rev. Anal. Chem. 2019 49 336 756-55-9602/10408347.2018.1531691 30596249 
13. Jung H.J.  Koutavarapu R.  Lee S.  Kim J.H.  Choi H.C.  Choi M.Y.   Enhanced photocatalytic degradation of lindane using metal–semiconductor Zn@ ZnO and ZnO/Ag nanostructures J. Environ. Sci. 2018 74 107 756-55-9602/j.jes.2018.02.014 30340663 
14. Khavar A.H.C.  Moussavi G.  Mahjoub A.R.  Luque R.  Rodríguez-Padrón D.  Sattari M.   Enhanced visible light photocatalytic degradation of acetaminophen with Ag2 S-ZnO@ rGO core-shell microsphere as a novel catalyst: Catalyst preparation and characterization and mechanistic catalytic experiments Sep. Purif. Technol. 2019 229 115756-55-9602/j.seppur.+1-945-404-0451 
15. Lee S.J.  Jung H.J.  Koutavarapu R.  Lee S.H.  Arumugam M.  Kim J.H.  Choi M.Y.   ZnO supported Au/Pd bimetallic nanocomposites for plasmon improved photocatalytic activity for methylene blue degradation under visible light irradiation Appl. Surf. Sci. 2019 496 143756-55-9602/j.apsusc.+1-945-404-0451 
16. Wang X.  Li Q.  Zhou C.  Cao Z.  Zhang R.   ZnO rod/reduced graphene oxide sensitized by α-Fe2 O3  nanoparticles for effective visible-light photoreduction of CO2  J. Colloid Interface Sci. 2019 554 335 756-55-9602/j.jcis.2019.07.014 31306945 
17. Taherkhani M.  Naderi N.  Fallahazad P.  Eshraghi M.J.  Kolahi A.   Development and Optical Properties of ZnO Nanoflowers on Porous Silicon for Photovoltaic Applications J. Electron. Mater. 2756-55-9602 6756-55-9602/s11664-019-07484-0 
18. Young S.-J.  Yuan K.-W.   ZnO Nanorod Humidity Sensor and Dye-Sensitized Solar Cells as a Self-Powered Device IEEE Trans. Electron Devices 2756-55-9602 3981 10.1109/TED.2019.2926021 
19. Zhang W.  Chang S.  Yao S.  Wang H.   Preparation and Characterization of Submicron Star-Like ZnO as Light Scattering Centers for Combination with ZnO Nanoparticles for Dye-Sensitized Solar Cells J. Electron. Mater. 2756-55-9602 4901 10.1007/s11664-019-07278-4 
20. Zhu L.  Chen C.  Weng Y.  Li F.  Lou Q.   Enhancing the performance of inverted perovskite solar cells by inserting a ZnO: TIPD film between PCBM layer and Ag electrode Sol. Energy Mater. Sol. Cells 2019 198 11 18 10.1016/j.solmat.2019.04.007 
21. Beyene Z.  Ghosh R.   Effect of zinc oxide addition on antimicrobial and antibiofilm activity of hydroxyapatite: A potential nanocomposite for biomedical applications Mater. Today Commun. 2756-55-960212 10.1016/j.mtcomm.+1-945-404-0451 
22. Feng J.N.  Guo X.P.  Chen Y.R.  Lu D.P.  Niu Z.S.  Tou F.Y.  Hou L.J.  Xu J.  Liu M.  Yang Y.   Time-dependent effects of ZnO nanoparticles on bacteria in an estuarine aquatic environment Sci. Total Environ. 2019 134756-55-9602/j.scitotenv.+1-945-404-0451 31505343 
23. Ghosh M.  Mandal S.  Roy A.  Chakrabarty S.  Chakrabarti G.  Pradhan S.K.   Enhanced antifungal activity of fluconazole conjugated with Cu-Ag-ZnO nanocomposite Mater. Sci. Eng. C 2019 110756-55-9602/j.msec.+1-945-404-0451 31753371 
24. Lozhkomoev A.  Kazantsev S.  Kondranova A.  Fomenko A.  Pervikov A.  Rodkevich N.  Bakina O.   Design of antimicrobial composite nanoparticles ZnxMe (100-x)/O by electrical explosion of two wires in the oxygen-containing atmosphere Mater. Des. 2019 183 108756-55-9602/j.matdes.+1-945-404-0451 
25. Chaudhary S.  Umar A.  Bhasin K.  Baskoutas S.   Chemical sensing applications of ZnO nanomaterials Materials 2018 11 756-55-9602/ma11020287 29439528 
26. Prabhu S.  Megala S.  Harish S.  Navaneethan M.  Maadeswaran P.  Sohila S.  Ramesh R.   Enhanced photocatalytic activities of ZnO dumbbell/reduced graphene oxide nanocomposites for degradation of organic pollutants via efficient charge separation pathway Appl. Surf. Sci. 2019 487 1279 1756-55-9602/j.apsusc.2019.05.086 
27. Segovia M.  Alegría M.  Aliaga J.  Celedon S.  Ballesteros L.  Sotomayor-Torres C.  González G.  Benavente E.   Heterostructured 2D ZnO hybrid nanocomposites sensitized with cubic Cu2 O nanoparticles for sunlight photocatalysis J. Mater. Sci. 2756-55-96023 13756-55-9602/s10853-019-03878-x 
28. Selvaraj S.  Mohan M.K.  Navaneethan M.  Ponnusamy S.  Muthamizhchelvan C.   Synthesis and photocatalytic activity of Gd doped ZnO nanoparticles for enhanced degradation of methylene blue under visible light Mater. Sci. Semicond. Process. 2019 103 104756-55-9602/j.mssp.+1-945-404-0451 
29. Shetti N.P.  Bukkitgar S.D.  Kakarla R.R.  Reddy C.  Aminabhavi T.M.   ZnO-based nanostructured electrodes for electrochemical sensors and biosensors in biomedical applications Biosens. Bioelectron. 2019 141 111756-55-9602/j.bios.+1-945-404-0451 31202187 
30. Taylor C.M.  Ramirez-Canon A.  Wenk J.  Mattia D.   Enhancing the Photo-corrosion Resistance of ZnO Nanowire Photocatalysts J. Hazard. Mater. 2019 378 120756-55-9602/j.jhazmat.+1-945-404-0451 31238260 
31. Umar A.  Kim S.  Kumar R.  Al-Assiri M.  Al-Salami A.  Ibrahim A.  Baskoutas S.   In-doped ZnO hexagonal stepped nanorods and nanodisks as potential scaffold for highly-sensitive phenyl hydrazine chemical sensors Materials 2756-55-9602 10.3390/ma10111337 29160823 
32. Khoa N.T.  Kim S.W.  Yoo D.-H.  Cho S.  Kim E.J.  Hahn S.H.   Fabrication of Au/graphene-wrapped ZnO-nanoparticle-assembled hollow spheres with effective photoinduced charge transfer for photocatalysis ACS Appl. Mater. Interfaces 2015 7 3524 3756-55-9602/acsami.5b00152 25629618 
33. Noman M.T.  Ashraf M.A.  Ali A.   Synthesis and applications of nano-TiO2 : A review Environ. Sci. Pollut. Res. 2756-55-9602 3756-55-9602/s11356-018-3884-z 30523526 
34. Noman M.T.  Ashraf M.A.  Jamshaid H.  Ali A.   A novel green stabilization of TiO2  nanoparticles onto cotton Fibers Polym. 2756-55-9602 2756-55-9602/s12221-018-8693-y 
35. Ong C.B.  Ng L.Y.  Mohammad A.W.   A review of ZnO nanoparticles as solar photocatalysts: Synthesis, mechanisms and applications Renew. Sustain. Energy Rev. 2018 81 536 756-55-9602/j.rser.2017.08.020 
36. Rehman S.  Jermy B.R.  Akhtar S.  Borgio J.F.  Abdul Azeez S.  Ravinayagam V.  Al Jindan R.  Alsalem Z.H.  Buhameid A.  Gani A.   Isolation and characterization of a novel thermophile; Bacillus haynesii, applied for the green synthesis of ZnO nanoparticles Artif. Cells Nanomed. Biotechnol. 2756-55-9602 2756-55-9602/21691401.2019.1620254 31126203 
37. Acosta-Humánez M.  Montes-Vides L.  Almanza-Montero O.   Sol-gel synthesis of zinc oxide nanoparticle at three different temperatures and its characterization via XRD, IR and EPR Dyna 2016 83 224 756-55-96026/dyna.v83n195.50833 
38. Jurablu S.  Farahmandjou M.  Firoozabadi T.   Sol-gel synthesis of zinc oxide (ZnO) nanoparticles: Study of structural and optical properties J. Sci. Islam. Repub. Iran 2015 26 281 285 
39. Konne J.L.  Christopher B.O.   Sol-gel syntheses of zinc oxide and hydrogenated zinc oxide (ZnO: H) phases J. Nanotechnol. 2017 2017 5219756-55-9602/2017/5219850 
40. Gong B.  Shi T.  Liao G.  Li X.  Huang J.  Zhou T.  Tang Z.   UV irradiation assisted growth of ZnO nanowires on optical fiber surface Appl. Surf. Sci. 2017 406 294 756-55-9602/j.apsusc.2017.02.153 
41. Ko R.-M.  Lin Y.-R.  Chen C.-Y.  Tseng P.-F.  Wang S.-J.   Facilitating epitaxial growth of ZnO films on patterned GaN layers: A solution-concentration-induced successive lateral growth mechanism Curr. Appl. Phys. 2018 18 1 11 10.1016/j.cap.2017.11.003 
42. Lu P.  Zhou W.  Li Y.  Wang J.  Wu P.   Abnormal room temperature ferromagnetism in CuO/ZnO nanocomposites via hydrothermal method Appl. Surf. Sci. 2017 399 396 756-55-9602/j.apsusc.2016.12.113 
43. Akhtari F.  Zorriasatein S.  Farahmandjou M.  Elahi S.M.   Synthesis and optical properties of Co2+ -doped ZnO Network prepared by new precursors Mater. Res. Express 2018 5 065756-55-9602/2053-1591/aac6f1 
44. Kumar K.M.  Mandal B.K.  Naidu E.A.  Sinha M.  Kumar K.S.  Reddy P.S.   Synthesis and characterisation of flower shaped zinc oxide nanostructures and its antimicrobial activity Spectrochim. Acta Part A Mol. Biomol. Spectrosc. 2013 104 171 756-55-9602/j.saa.2012.11.025 23266691 
45. Lanje A.S.  Sharma S.J.  Ningthoujam R.S.  Ahn J.-S.  Pode R.B.   Low temperature dielectric studies of zinc oxide (ZnO) nanoparticles prepared by precipitation method Adv. Powder Technol. 2013 24 331 756-55-9602/j.apt.2012.08.005 
46. Dobrucka R.  Długaszewska J.   Biosynthesis and antibacterial activity of ZnO nanoparticles using Trifolium pratense flower extract Saudi J. Biol. Sci. 2016 23 517 756-55-9602/j.sjbs.2015.05.016 27298586 
47. Jamdagni P.  Khatri P.  Rana J.   Green synthesis of zinc oxide nanoparticles using flower extract of Nyctanthes arbor-tristis and their antifungal activity J. King Saud Univ. Sci. 2018 30 168 756-55-9602/j.jksus.2016.10.002 
48. Mirzaei H.  Darroudi M.   Zinc oxide nanoparticles: Biological synthesis and biomedical applications Ceram. Int. 2017 43 907 914 10.1016/j.ceramint.2016.10.051 
49. Slman D.K.  Jalill R.D.A.  Abd A.N.   Biosynthesis of zinc oxide nanoparticles by hot aqueous extract of Allium sativum plants J. Pharm. Sci. Res. 2756-55-9602 1596 
50. Pant B.  Ojha G.P.  Kim H.-Y.  Park M.  Park S.-J.   Fly-ash-incorporated electrospun zinc oxide nanofibers: Potential material for environmental remediation Environ. Pollut. 2019 245 163 756-55-9602/j.envpol.2018.10.122 30419457 
51. Pant B.  Park M.  Kim H.-Y.  Park S.-J.   Ag-ZnO photocatalyst anchored on carbon nanofibers: Synthesis, characterization, and photocatalytic activities Synth. Met. 2016 220 533 756-55-9602/j.synthmet.2016.07.027 
52. Ezeh C.I.  Yang X.  He J.  Snape C.  Cheng X.M.   Correlating ultrasonic impulse and addition of ZnO promoter with CO2  conversion and methanol selectivity of CuO/ZrO2  catalysts Ultrason. Sonochem. 2018 42 48 56 10.1016/j.ultsonch.2017.11.013 29429694 
53. Sebastian N.  Yu W.-C.  Hu Y.-C.  Balram D.  Yu Y.-H.   Sonochemical synthesis of iron-graphene oxide/honeycomb-like ZnO ternary nanohybrids for sensitive electrochemical detection of antipsychotic drug chlorpromazine Ultrason. Sonochem. 2756-55-960296 10.1016/j.ultsonch.+1-945-404-0451 31430655 
54. Noman M.T.  Wiener J.  Saskova J.  Ashraf M.A.  Vikova M.  Jamshaid H.  Kejzlar P.   In-situ development of highly photocatalytic multifunctional nanocomposites by ultrasonic acoustic method Ultrason. Sonochem. 2018 40 41 56 10.1016/j.ultsonch.2017.06.026 28946440 
55. Pholnak C.  Sirisathitkul C.  Danworaphong S.  Harding D.J.   Sonochemical synthesis of zinc oxide nanoparticles using an ultrasonic homogenizer Ferroelectrics 2013 455 15 20 10.1080/00150193.2013.843405 
56. Luévano-Hipólito E.  Torres-Martínez L.   Sonochemical synthesis of ZnO nanoparticles and its use as photocatalyst in H2  generation Mater. Sci. Eng. B 2017 226 223 756-55-9602/j.mseb.2017.09.023 
57. Ma Q.L.  Xiong R.  Zhai B.G.  Huang Y.M.   Ultrasonic synthesis of fern-like ZnO nanoleaves and their enhanced photocatalytic activity Appl. Surf. Sci. 2015 324 842 756-55-9602/j.apsusc.2014.11.054 
58. Mahmoodi N.M.  Keshavarzi S.  Ghezelbash M.   Synthesis of nanoparticle and modelling of its photocatalytic dye degradation ability from colored wastewater J. Environ. Chem. Eng. 2017 5 3684 3756-55-9602/j.jece.2017.07.010 
59. Dhiman N.  Singh A.  Verma N.K.  Ajaria N.  Patnaik S.   Statistical optimization and artificial neural network modeling for acridine orange dye degradation using in-situ synthesized polymer capped ZnO nanoparticles J. Colloid Interface Sci. 2017 493 295 756-55-9602/j.jcis.2017.01.042 28119240 
60. Rodrigues J.  Hatami T.  Rosa J.M.  Tambourgi E.B.  Mei L.H.I.   Photocatalytic degradation using ZnO for the treatment of RB 19 and RB 21 dyes in industrial effluents and mathematical modeling of the process Chem. Eng. Res. Des. 2020 153 294 756-55-9602/j.cherd.2019.10.021 
61. Noman M.T.  Militky J.  Wiener J.  Saskova J.  Ashraf M.A.  Jamshaid H.  Azeem M.   Sonochemical synthesis of highly crystalline photocatalyst for industrial applications Ultrasonics 2018 83 203 756-55-9602/j.ultras.2017.06.012 28655399 
62. Schneider J.R.J.  Hoffmann R.C.  Engstler J.R.  Klyszcz A.  Erdem E.  Jakes P.  Eichel R.D.-A.  Pitta-Bauermann L.  Bill J.   Synthesis, characterization, defect chemistry, and FET properties of microwave-derived nanoscaled zinc oxide Chem. Mater. 2756-55-9602 2756-55-9602/cm902300q 
63. Rakhshaei R.  Namazi H.  Hamishehkar H.  Kafil H.S.  Salehi R.   In situ synthesized chitosan–gelatin/ZnO nanocomposite scaffold with drug delivery properties: Higher antibacterial and lower cytotoxicity effects J. Appl. Polym. Sci. 2019 136 47756-55-9602/app.47590


{'source': 'PubMedDataset'}